Calculating anisotropic physical properties from texture data using the MTEX open source package


 Harriet Houston
 1 years ago
 Views:
Transcription
1 Calculating anisotropic physical properties from texture data using the MTEX open source package David Mainprice 1, Ralf Hielscher 2, Helmut Schaeben 3 February 10, Geosciences Montpellier UMR CNRS 5243, Université Montpellier 2, Montpellier Cedex 05, France 2 Fakultät für Mathematik, Technische Universität Chemnitz, Chemnitz, Germany Mathematische Geologie und Geoinformatik, Institut für Geophysik und Geoinformatik, Technische Universität Freiberg, Freiberg, Germany submitted to Deformation Mechanism, Rheology & Tectonics: Microstructures, Mechanics & Anisotropy  The Martin Casey Volume. In: Prior, D., Rutter, E.H., Tatham, D. J. (eds) Geological Society of London, Special Publication REVISED VERSION 8/02/2011 DM Abstract This paper presents the theoretical background for the calculation of physical properties of an aggregate from constituent crystal properties and the texture of the aggregate in a coherent manner. Emphasis is placed on the important tensor properties of 2 nd and 4 th rank with applications in rock deformation, structural geology, geodynamics and geophysics. We cover texture information that comes from pole figure diffraction and single orientation measurements (Electron Backscattered Diffraction, Electron Channeling Pattern, Laue Pattern, Optical microscope universalstage). In particular, we give explicit formulas for the calculation of the averaged tensor from individual orientations or from an ODF. For the latter we consider numerical integration and an approach based on the expansion into spherical harmonics. This paper also serves as a reference paper for the tensor mathematic capabilities of the texture analysis software MTEX, which is a comprehensive, freely available MATLAB toolbox that covers a wide range of problems in quantitative texture analysis, e.g. orientation distribution function (ODF) modeling, pole figure to ODF inversion, EBSD data analysis, and grain detection. MTEX offers a programming interface, which allows the processing of involved research problems, as well as highly customizable visualization capabilities, which makes it perfect for scientific presentations, publications and teaching demonstrations. Keywords: physical properties, tensors, texture, orientation density function, crystallographic preferred orientation, averaging methods, EBSD 1
2 Introduction The estimation of physical properties of crystalline aggregates from the properties of the component crystals has been subject of extensive literature since the classical work of Voigt (1928) and Reuss (1929). Such an approach is only feasible if the bulk properties of the crystals dominate the physical property of the aggregate and the effects of grain boundary interfaces can be ignored. For example, the methods discussed here cannot be applied to the electrical properties of watersaturated rock, where the role of interfacial conduction is likely to be important. Many properties of interest to earth and materials scientists can be evaluated from the knowledge of the single crystal tensors and the orientation distribution function (ODF) of crystals in an aggregate, for example thermal diffusivity, thermal expansion, diamagnetism and elastic wave velocities. The majority of rockforming minerals have strongly anisotropic physical properties and many rocks also have strong crystal preferred orientations (CPOs, or textures as they are called in Materials Science) that can be described concisely in a quantitative manner by the orientation density function ODF. The combination of strong CPOs and anisotropic single crystal properties results in a three dimensional variation in rock properties. Petrophysical measurements are usually made under hydrostatic pressure, and often at high temperature to simulate conditions in the Earth, where presumably the microcracks present at ambient conditions are closed. The necessity to work at high pressure and temperature conditions limits the number of orientations that can be measured. Typically, three orthogonal directions are measured parallel to structural features, such as the lineation and foliation normal defined by grain shape. The evaluation of physical properties from CPO allows the determination of properties over the complete orientation sphere of the specimen reference frame. This paper is designed as a reference paper for earth and material scientists who want to use the texture analysis software MTEX to compute physical tensor properties of aggregates from constituent crystal properties and the texture of the aggregate. MTEX is a comprehensive, freely available MATLAB toolbox that covers a wide range of problems in quantitative texture analysis, e.g. ODF modeling, pole figure to ODF inversion, EBSD data analysis, and grain detection. The MTEX toolbox can be downloaded from Unlike many other texture analysis software, it offers a programming interface, which allows for the efficient processing of complex research problems in the form of scripts (Mfiles). The MATLAB environment provides a wide variety of high quality graphics file format to aid publication and display of the results. In addition the MTEX toolbox will work identically on Microsoft Windows, Apple Mac OSX and Linux platforms in 32 and 64 bit modes with a simple installation procedure. In MTEX texture analysis information like ODFs, EBSD data, pole figures, are represented by variables of different types. For example, in order to define a unimodal ODF with halfwidth 10, preferred orientation (10, 20, 30 ) Euler angles and cubic crystal symmetry, one issues the command myodf = unimodalodf( orientation ( Euler,10 degree,20 degree,30 degree ),... symmetry( c u b i c ), h a l f w i d t h,10 degree ) 2
3 which generates a variable myodf of type ODF which is displayed as myodf = ODF specimen symmetry : triclinic crystal symmetry : cubic Radially symmetric portion : kernel : de la Vallee Poussin, hw = 10 center : (10,20,30) weight : 1 We will keep this style of displaying input and output to make the syntax of MTEX as clear as possible. Note that there is also an exhaustive interactive documentation included in MTEX, which explains the syntax of each command in detail. The outline of the paper is as follows. In the first section the basics of tensors mathematics and crystal geometry are briefly mentioned and presented in terms of MTEX commands. In the second section these basics are discussed for some classical second order tensors and the elasticity tensors. In particular we give a comprehensive overview about elastic properties that can be computed directly from the elastic stiffness tensor. All calculations are accompanied by the corresponding MTEX commands. In the third section we are concerned with the calculation of average matter tensors from their single crystal counterparts and the texture of the aggregate. Here we consider textures given by individual orientation measurements, which leads to the well known Voigt, Reuss, and Hill averages, as well as textures given by ODFs, which leads to formulas involving integrals over the orientation space. We can compute these integrals in several ways. Either we use known quadrature rule, or we compute the expansion of the rotated tensor into generalized spherical harmonics and apply Parseval s theorem. Explicit formulae for the expansion of a tensor into generalized spherical harmonics and a proof that the order of the tensor defines the maximum order of this expansion is included in the appendix. 2 Tensor mathematics and crystal geometry In what follows we give the necessary background to undertake physical property calculation for single crystals, without necessarily the full mathematical developments that can be found elsewhere (e.g. Nye, 1985). We will restrict ourselves to linear physical properties, that are properties than can be described by a linear relationship between cause and effect, such as stress and strain for linear elasticity. 2.1 Tensors Mathematically, a tensor T of rank r is a r linear mapping which can be represented by an r dimensional matrix T i1,i 2,...,i r. Thus a rank zero tensor is simply a scalar value, a rank one tensor T i is a vector, and a rank two tensor T ij has the form of a matrix. Linearity 3
4 means that the tensor applied to r vectors x 1,..., x r R 3, defines a mapping (x 1,..., x r ) T i1,...,i r x 1 i 1 x r i r i 1 =1 i 2 =1 i r=1 98 which is linear in each of the arguments x 1,..., x r. Physically, tensors are used to described linear interactions between physical properties. In the simplest case, scalar properties are modelled by rank zero tensor, whereas vector fields, i.e., direction dependent properties, are modelled by rank one tensors. An example for a second rank tensor is the thermal conductivity tensor k ij which describes the lineral relationship between the negative temperature gradient gradt = ( T x 1, T x 2, T x 3 ), i.e. a first order tensor, and the heat flux q = (q 1, q 2, q 3 ) per unit area which is also an first order tensor. The linear relationship is given by the equality q i = 3 j=1 k ij T x j, i = 1,..., 3, and can be seen as a matrix vector product of the thermal conductivity tensor k ij interpreted as a matrix and the negative temperature gradient interpreted as a vector. In the present example the negative temperature gradient is called applied tensor and the heat flux is called induced tensor. In the general case, we define a rank r tensor T i1,...,i r, inductively, as the linear relationship between two physical properties which are modelled by a rank s tensor A j1,j 2,...,j s and a rank t tensor B k1,k 2,...,k t, such that the equation r = t + s is satisfied. So the rank of a tensor is given by the rank of the induced tensor plus the rank of the applied tensor. The linear dependency between the applied tensor A and the induced tensor B is given by the tensor product B k1,...,k t = T k1,k 2,...,k t,j 1,...,j s A j1,...,j s = T k1,k 2,...,k t,j 1,...,j s A j1,...,j s j 1 =1 j 1 =1 j s= In the right hand side of the last equation we used the Einstein summation convention and omitted the sum sign for every two equal indexes. This will be default in all further formulae. In MTEX a tensor is represented by a variable of type tensor. In order to create such a variable, the r dimensional matrix has to be specified. As an example we consider the 2 nd rank stress tensor σ ij, which can be defined by M = [ [ ] ;... [ ] ;... [ ] ] ; sigma = tensor (M, name, s t r e s s, u n i t, MPa ) ; 4
5 sigma = stress tensor ( size : 3 3) rank : 2 unit : MPa Furthermore, we defined the normal n = (1, 0, 0) to plane by n = vector3d ( 1, 0, 0 ) n = vector3d ( size : 1 1) x y z Then according to Cauchy s stress principle the stress vector T n associated with the plane normal n, is computed by T n j = σ ij n i. In MTEX this equation may be written as T = EinsteinSum ( sigma,[ 1 1 ], n, 1, u n i t, MPa ) T = tensor ( size : 3) unit : MPa rank : Note that the 1 in the arguments of the command EinsteinSum indicates the dimension which has to be summed up and the 1 in the argument indicates that the second dimension of σ becomes the first dimension of T. Using the stress vector T n the scalar magnitudes of the normal stress σ N and the shear stress σ S are given as σ N = T n i n i = σ ij n i n j and σ S = In MTEX the corresponding calcuation reads as T n i T n i σ 2 N. sigman = double ( EinsteinSum (T, 1,n, 1)) sigmas = sqrt ( double ( EinsteinSum (T, 1,T, 1)) sigman ˆ2) sigman = sigmas =
6 crystal symmetries X T Y T Z T orthorhombic, tetragonal, cubic a b c trigonal, hexagonal a m c m a c monoclinic a b c a b c triclinic a Z T X T c a Z T X T c Y T Z T b c Y T Z T b c Table 1: Alignment of the crystal reference frame for the tensors of physical properties of crystals. The letters a, b, c, m correspond to crystallographic directions in the direct lattice space, whereas the letters a, b, c denote the corresponding directions in the reciprocal lattice space, which are parallel to the normal to the plane written as a for a etc. N.B. there are atleast two possible reference choices for all symmetries except orthorhombic, tetragonal and cubic The crystal reference frame Tensors can be classified into two types: matter tensors describing physical properties like electrical or thermal conductivity, magnetic permeability, etc., of a crystalline specimen, and field tensors describing applied forces, like stress, strain, or a electric field, to a specimen. Furthermore, it is important to distinguish between single crystal tensors describing constituent crystal properties and tensors describing averaged macroscopic properties of a polycrystalline specimen. While the reference frame for the latter ones is the specimen coordinate system, the reference frame for single crystal tensor properties is unambiguously connected with the crystal coordinate system. The reference frames and their conventions are explained below. We will restrict ourselves to tensors of single or polycrystals defined in a Cartesian reference frame comprising 3 unit vectors, X T, Y T, Z T. The use of an orthogonal reference frame for single crystals avoids the complications of the metric associated with the crystal unit cell axes. In any case, almost all modern measurements of physical property tensors are reported using Cartesian reference frames. Next we discuss how the single crystal tensor reference frame is defined using the crystal coordinate system. In the general case of triclinic crystal symmetry, the crystal coordinate system is specified by its axis lengths a, b, c and interaxial angles α, β, γ resulting in a non Euclidean coordinate system a, b, c for the general case. In order to align the Euclidean tensor reference frame X T, Y T, Z T in the crystal coordinate system several conventions are in use. The most common ones are summarized in Table 1. In MTEX the alignment of the crystal reference frame is defined together with the symmetry group and the crystal coordinate system. All this information is stored in a variable 6
7 of type symmetry. For example by c s t e n s o r = symmetry( t r i c l i n i c, [ , , ],... [ , , ] degree, X a, Z c, mineral, Talc ) ; cs_ tensor = symmetry ( size : 1) mineral : Talc symmetry : triclinic ( 1) a, b, c : 5.3, 9.2, 9.4 alpha, beta, gamma : 90.4, 98.9, reference frame : X a*, Z c we store in the variable cs tensor the geometry of Talc which has triclinic crystal symmetry, axes length 5.29, 9.18, 9.42, inter axial angles 90.4, 98.9, 90.1, and the convention for a Cartesian righthanded tensor reference frame X a, Z c and hence Y = Z X for the alignment of the crystal reference frame. In order to define a crystal constituent property tensor with respect to this crystal reference frame we append the variable cs tensor to its definition, i.e., M = [ [ ] ;... [ ] ;... [ ] ;... [ ] ;... [ ] ;... [ ] ] ; C = tensor (M, name, e l a s t i c s t i f f n e s s, unit, GPa, c s t e n s o r ) C = elastic stiffness tensor ( size : ) unit : GPa rank : 4 mineral : Talc ( triclinic, X a*, Z c) tensor in Voigt matrix representation defines the elastic stiffness tensor in GPa of Talc. This example will be discussed in greater detail in section Crystal Orientations Let X c, Y c, Z c be a Euclidean crystal coordinate system assigned to a specific crystal and let X s, Y s, Z s a specimen coordinate system. Then in general, in polycrystalline materials the two coordinate systems do not coincide. Their relative alignment describes the orientation of the crystal within the specimen. More specifically, the orientation of a crystal is defined 7
8 as the (active) rotation g that rotates the specimen coordinate system into coincidence with the crystal coordinate system. From another point of view, the rotation g can be described as the basis transformation from the crystal coordinate system to specimen coordinate system. Let h = (h 1, h 2, h 3 ) be the coordinates of a specific direction with respect to the crystal coordinate system. Then r = (r 1, r 2, r 3 ) = g h are the coordinates of the same direction with respect to the specimen coordinate system. Crystal orientations are typically defined by Euler angles, either by specifying rotations with angles φ 1, Φ, φ 2 about the axes Z s, X s, Z s (Bunge convention), or with angles α, β, γ about the axes Z s, Y s, Z s (Matthies convention). In MTEX both conventions, and also some others, are supported. In order to define an orientation in MTEX we start by fixing the crystal reference frame X c, Y c, Z c used for the definition of the orientation, c s o r i e n t a t i o n = symmetry( t r i c l i n i c, [ , , ], [ , , ] degree,... X a, Z c, mineral, Talc ) ; cs_ orientation = crystal symmetry ( size : 1) mineral : Talc symmetry : triclinic ( 1) a, b, c : 5.3, 9.2, 9.4 alpha, beta, gamma : 90.4, 98.9, reference frame : X a, Z c* Now an orientation can be defined as a variable of type orientation, g = orientation ( Euler,10 degree,20 degree, 5 degree, Bunge, c s o r i e n t a t i o n ) g = orientation ( size : 1 1) mineral : Talc crystal symmetry : triclinic, X a, Z c* specimen symmetry : triclinic Bunge Euler angles in degree phi1 Phi phi Note, that for the definition of an orientation the crystal reference frame is crucial. Therefore, the definition of the variable of type orientation necessarily includes a variable of type symmetry, storing the relevant information. This applies, in particular, if the orientation data, i.e. Euler angles, are imported from third party measurement systems, such as EBSD, and associated software with their own specific conventions for X c, Y c, Z c, which should be defined when using the MTEX import wizard. In order to demonstrate the coordinate transform between the crystal and the specimen coordinate system, we choose a crystal direction in the reciprocal lattice h = h a +kb +lc (pole to a plane) by defining a variable of type Miller h = Miller ( 1, 1, 0, c s o r i e n t a t i o n, h k l ) h = Miller ( size : 1 1) mineral : Talc ( triclinic, X a, Z c*) 8
9 h 1 k 1 l 0 and express it in terms of the specimen coordinate system for a specific orientation g = (10, 20, 5 ) r = g h r = vector3d ( size : 1 1), x y z The resulting variable is of type vector3d reflecting that the new coordinate system is the specimen coordinate system. Note, that in order that the coordinate transformation rule makes sense physically, the corresponding crystal reference frames used for the definition of the orientation and the crystal direction by Miller indices must coincide. Alternatively, one can specify a crystal direction u = u a + v b + w c in direct space u = Miller ( 1, 1, 0, c s o r i e n t a t i o n, uvw ) u = Miller ( size : 1 1), uvw mineral : Talc ( triclinic, X a, Z c*) u 1 v 1 w 0 and express it in terms of the specimen coordinate system r = g u r = vector3d ( size : 1 1), x y z Obviously, this gives a different direction, since direct and reciprocal space do not coincide for triclinic crystal symmetry. 2.4 The relationship between the single crystal physical property and Euler angle reference frames Let us consider a rank r tensor T i1,...,i r describing some physical property of a crystal with respect to a well defined crystal reference frame X T, Y T, Z T. Then one is often interested in expressing the tensor with respect to another, different Euclidean reference frame X, Y, Z, which might be 1. a crystallographically equivalent crystal reference frame, 2. a different convention for aligning the Euclidean reference frame to the crystal coordinate system, or, 9
10 a specimen coordinate system. Let us first consider a vector h that has the representation h = h T 1 X T + h T 2 Y T + h T 3 X T with respect to the tensor reference frame X T, Y T, Z T, and the representation h = h1 X + h2 Y + h3 X. with respect to the other reference frame X, Y, Z. Then the coordinates h T 1, h T 2, h T 3 and h 1, h 2, h 3 satisfy the transformation rule h 1 X X T X Y T X Z T h T h 2 = Y X T 1 Y Y T Y Z T, (1) h 3 Z X T Z Y T Z Z T } {{ } =:R i.e., the matrix R performs the coordinate transformation from the tensor reference frame X T, Y T, Z T to the other reference frame X, Y, Z. The matrix R can be also interpreted as the rotation matrix that rotates the second reference frame into coincidence with the tensor reference frame. Considering h T j to be a rank one tensor, the transformation rule becomes h i = h T j R ij. This formula generalizes to arbitrary tensors. Let Ti T 1,...,i r be the coefficients of a rank r tensor with respect to the crystal reference frame X T, Y T, Z T and let T i1,...,i r be the coefficients with respect to another reference frame X, Y, Z. Then the linear orthogonal transformation law for Cartesian tensors states the relationship T i1,...,i r = T T j 1,...,j r R i1 j 1 R irj r. (2) h T 2 h T Let us now examine the three cases for a new reference frame as mentioned at the beginning of this section. In the case of a crystallographically equivalent reference frame the coordinate transform R is a symmetry element of the crystal and the tensor remains invariant with respect to this coordinate transformation, i.e. Ti1,...,i r = T i1,...,i r. In the case that the other reference frame X, Y, Z follows a different convention in aligning to the crystal coordinate system the transformed tensor T i1,...,i r is in general different to the original one. In MTEX this change of reference frame is done by the command set. Let us consider the elastic stiffness tensor C ijkl of Talc as defined above C = elastic stiffness tensor ( size : ) unit : GPa rank : 4 mineral : Talc ( triclinic, X a*, Z c)
11 and let us consider the reference frame cs orientation as defined in the previous section cs_ orientation = Symmetry ( size : 1) mineral : Talc symmetry : triclinic ( 1) a, b, c : 5.29, 9.18, 9.42 alpha, beta, gamma : 90.4, 98.9, reference frame : X a, Z c* Then the elastic stiffness tensor C ijkl of Talc with respect to the reference frame cs orientation is computed by setting cs orientation as the new reference frame C o r i e n t a t i o n = set (C, CS, c s o r i e n t a t i o n ) C_ orientation = elastic stiffness tensor ( size : ) unit : GPa rank : 4 mineral : Talc ( triclinic, X a, Z c*) tensor in Voigt matrix representation Finally, we consider the case that the second reference frame is not aligned to the crystal coordinate system, but to the specimen coordinate system. Then, according to the previous section, the coordinate transform defines the orientation g of the crystal and equation (2) tells us how the tensor has to be rotated according to the crystal orientation. In this case we will write T i1,...,i r = T T j 1,...,j r (g) = T T j 1,...,j r R i1 j 1 (g) R irj r (g), (3) to express the dependency of the resulting tensor from the orientation g. Here R irjr (g) is the rotation matrix defined by the orienation g. It is of major importance, in order to apply formula (3), that both, the tensor reference frame and the crystal reference frame used for describing the orientation coincide. If they do not coincide, the tensor has to be transformed to the same crystal reference frame used for describing the orientation. Hence, when working with tensors and orientation data it is always necessary to know the tensor reference frame and the crystal reference frame used for describing the orientation. In practical applications this is not always a simple task, as those information are sometimes hidden by the commercial EBSD systems. 11
12 If the corresponding reference frames are specified in the definition of the tensor as well as in the definition of the orientation, MTEX automatically checks for coincidence and performs the necessary coordinate transforms if they do not coincide. Eventually, the rotated tensor for an orientation g = (10, 20, 5 ) is computed by the command rotate, C rotated = rotate (C, g ) C_ rotated = elastic_ stiffness tensor ( size : ) unit : GPa rank : 4 tensor in Voigt matrix representation Note, that the resulting tensor does not contain any information on the original mineral or reference frame. This is because the single crystal tensor is now with respect to the specimen coordinate system and can be averaged with any other elastic stiffness tensor from any other crystal of any composition and orientation Single crystal anisotropic properties Next we present some classical properties of single crystals that can be described by tensors (cf. Nye, 1985). 3.1 Second Rank Tensors A typical second rank tensor describes the relationship between an applied vector field and an induced vector field, such that the induced effect is equal to the tensor property multiplied by the applied vector. Examples of such a tensor are the electrical conductivity tensor, where the applied electric field induces a field of current density, the dielectric susceptibility tensor, where the applied electric field intensity induces electric polarization, the magnetic susceptibility tensor, where the applied magnetic field induces the intensity of magnetization, the magnetic permeability tensor, where the applied magnetic field induces magnetic induction, 12
13 the thermal conductivity tensor, where the applied negative temperature gradient induces heat flux. As a typical example for a second rank tensor we consider the thermal conductivity tensor k, k 11 k 12 k 13 x 1 q T 1 x 2 q T 1 x 2 q T 1 k = k 21 k 22 k 23 = x 1 q T 2 x 2 q T 2 x 2 q T 2 k 31 k 32 k 33 x 1 q T 3 x 2 q T 3 x 2 q T 3 which relates the negative temperature gradient gradt = ( T flux q = (q 1, q 2, q 3 ) per unit area by q i = 3 j=1 x 1, T x 2, T x 3 ) with the heat k ij T x j = k ij T x j. (4) In the present example the applied vector is the negative temperature gradient and the induced vector is the heat flux. Furthermore, we see that the relating vector is built up as a matrix, where the applied vector is the denominator of the rows and the induced vector is the numerator of columns. We see that the tensor entries k ij describe the heat flux q i in direction X i given a thermal gradient T x j in direction X j. As an example we consider the thermal conductivity of monoclinic orthoclase (Hofer and Schilling, 2002). We start by defining the tensor reference frame and the tensor coefficients in W m 1 K 1. c s t e n s o r = symmetry( monoclinic, [ , , ], [ 9 0, , 90] degree,... mineral, o r t h o c l a s e, Y b, Z c ) ; M = [ [ ] ;... [ ] ;... [ ] ] ; Now the thermal conductivity tensor k is defined by k = tensor (M, name, thermal c o n d u c t i v i t y, u n i t, W 1/m 1/K, c s t e n s o r ) k = thermal conductivity tensor ( size : 3 3) unit : W 1/ m 1/ K rank : 2 mineral : orthoclase ( monoclinic, X a*, Y b, Z c) Using the thermal conductivity tensor k we can compute the thermal flux q in W m 2 for a temperature gradient in Km 1 gradt = Miller ( 1, 1, 0, c s t e n s o r, uvw ) 13
14 gradt = Miller ( size : 1 1), uvw mineral : Orthoclase ( monoclinic, X a*, Y b, Z c) u 1 v 1 w 0 by equation (4), which becomes in MTEX q = EinsteinSum ( k, [ 1 1], gradt, 1, name, thermal f l u x, u n i t, W 1/mˆ2 ) q = thermal flux tensor ( size : 3) unit : W 1/ m ^2 rank : 1 mineral : orthoclase ( monoclinic, X a*, Y b, Z c) Note that the 1 in the arguments of the command EinsteinSum indicates the dimension which has to be summed up and the 1 in the argument indicates that the first dimension of k becomes the first dimension of q, see equation (4) A second order tensor k ij can be visualized by plotting its magnitude R( x) in a given direction x, R( x) = k ij x i x j. In MTEX the magnitude in a given direction x can be computed via x = Miller ( 1, 0, 0, c s t e n s o r, uvw ) ; R = EinsteinSum ( k,[ 1 2],x, 1,x, 2) R = tensor ( size : ) rank : 0 mineral : orthoclase ( monoclinic, X a*, Y b, Z c) Again the negative arguments 1 and 2 indicates which dimensions have to be multiplied and summed up. Alternatively, one can use the command magnitude, R = d i r e c t i o n a l M a g n i t u d e ( k, x ) Since in MTEX the directional magnitude is the default output of the plot command, the code plot ( k ) colorbar plots the directional magnitude of k with respect to any direction x as shown in Figure 1. Note that, by default, the X axis is plotted in north direction, the Y is plotted in west direction, and the Z axis is at the center of the plot. This default alignment can be changed by the commands plotx2north, plotx2east, plotx2south, plotx2west. 14
15 When the tensor k is rotated the directional magnitude rotates accordingly. This can be checked in MTEX by g = orientation ( Euler,10 degree,20 degree,30 degree, c s t e n s o r ) ; k r o t = rotate ( k, g ) ; plot ( k r o t ) The resulting plot is shown in Figure 1. From the directional magnitude we observe, furthermore, that the thermal conductivity tensor k is symmetric, i.e., k ij = k ji. This implies, in particular, that the thermal conductivity is an axial or nonpolar property, which means that the magnitude of heat flow is the same in positive or negative crystallographic directions. X Y Z min: 1.37 max: min: 1.37 max: Figure 1: The thermal conductivity k of Orthoclase visualized by its directionally varying magnitude for the tensor in standard orientation (left plot) and for the rotated tensor (right plot). We want to emphasize that there are also second rank tensors, which do not describe the relationship between an applied vector field and and an induced vector field, but relates, for instance, a zero rank tensor to a second rank tensor. The thermal expansion tensor α, α ij = ε ij T, is an example of such a tensor which relates a small applied temperature change T, which is a scalar, i.e., a zero rank tensor, to the induced strain tensor ε ij, which is a second rank tensor. The corresponding coefficient of volume thermal expansion becomes 1 V V T = α ii. This relationship holds true only for small changes in temperature. For larger changes in temperature, higher order terms have to be considered (see Fei, 1995 for data on minerals). This also applies to other tensors. 15
16 Elasticity Tensors We will now present fourth rank tensors, but restrict ourselves to the elastic tensors. Let σ ij be the second rank stress tensor and let ε kl be the second rank infinitesimal strain tensor. Then the fourth rank elastic stiffness tensor C ijkl describes the stress σ ij induced by the strain ε kl, i.e., it is defined by the equality σ ij = C ijkl ε kl, (5) which is known as Hooke s law for linear elasticity. Alternatively, the fourth order elastic compliance tensor S ijkl describes the strain ε kl induced by the stress σ ij, i.e., it is defined by the equality ε kl = S ijkl σ ij. The above definitions may also be written as the equalities C ijkl = σ ij ε kl and S ijkl = ε kl σ ij. In the case of static equilibrium for the stress tensor and infinitesimal deformation for the strain tensor, both tensors are symmetric, i.e., σ ij = σ ji and ε ij = ε ji. This implies for the elastic stiffness tensor the symmetry C ijkl = C ijlk = C jikl = C jilk, reducing the number of independent entries of the tensor from 3 4 = 81 to 36. Since, the elastic stiffness C ijkl is related to the internal energy U of a body, assuming constant entropy, by C ijkl = ( ) U, ε kl we obtain by Schwarz integrability condition C ijkl = ( ) ( ) ( ) U 2 U 2 U = = = C klij. ε kl ε ij ε ij ε kl ε kl ε ij Hence, ε ij C ijkl = C klij, which further reduces the number of independent entries from 36 to 21 ( e.g. Mainprice, 2007). These 21 independent entries may be efficiently represented in from of a symmetric 6 6 matrix C mn, m, n = 1,..., 6 as introduced by Voigt (1928). The entries C mn of this matrix representation equal the tensor entries C ijkl whenever m and n correspond to ij and kl according to the following table. m or n ij or kl , 32 13, 31 12, 21 16
17 The Voigt notation is used for published compilations of elastic tensors (e.g. Bass, 1995, Isaak, 2001). In a similar manner a Voigt representation S mn is defined for the elastic compliance tensor S ijkl. However, there are additional factors when converting between the Voigt S mn matrix representation and the tensor representation S ijkl. More precisely, we have for all ij, kl, m, n which correspond to each other according to the above table the identities: P = 1, if both m, n = 1, 2, 3 S ijkl = P S mn, P = 1, if either m or n are 4, 5, 6 2 P = 1, if both m, n = 4, 5, 6 4 Using the Voigt matrix representation of the elastic stiffness tensor equation (5) may be written as σ 11 C 11 C 12 C 13 C 14 C 15 C 16 ε 11 σ 22 C 21 C 22 C 23 C 24 C 25 C 26 ε 22 σ 33 σ 23 = C 31 C 32 C 33 C 34 C 35 C 36 ε 33 C 41 C 42 C 43 C 44 C 45 C 46 2ε 23. σ 13 σ 12 C 51 C 52 C 53 C 54 C 55 C 56 C 61 C 62 C 63 C 64 C 65 C 66 2ε 13 2ε 12 The matrix representation of Hooke s law allows for a straightforward interpretation of the tensor coefficients C ij. E.g., the tensor coefficient C 11 describes the dependency between normal stress σ 11 in direction X and axial strain ε 11 in the same direction. The coefficient C 14 describes the dependency between normal stress σ 11 in direction X and shear strain 2ε 23 = 2ε 32 in direction Y in the plane normal to Z. The dependency between normal stress σ 11 and axial strains ε 11, ε 22, ε 33, along X, Y and Z is described by C 11, C 12 and C 13, whereas the dependecies between the normal stress σ 11 and shear strains 2ε 23, 2ε 13 and 2ε 12 are described by C 14, C 15 and C 16. These effects are most important in low symmetry crystals, such as triclinic and monoclinic crystals, where there are a large number of nonzero coefficients. In MTEX the elasticity tensors may be specified directly in Voigt notation as we have already seen in Section 2.2. Alternatively, tensors may also be imported from ASCII files using a graphical interface called import wizard in MTEX. Let C be the elastic stiffness tensor for Talc in GPa as defined in Section 2.2. C = elastic_ stiffness tensor ( size : ) unit : GPa rank : 4 mineral : Talc ( triclinic, X a*, Z c) tensor in Voigt matrix representation
18 Then the elastic compliance S in GPa 1 can be computed by inverting the tensor C. S = inv (C) S = elastic compliance tensor ( size : ) unit : 1/ GPa rank : 4 mineral : Talc ( triclinic, X a*, Z c) tensor in Voigt matrix representation e e e e Elastic Properties The fourth order elastic stiffness tensor C ijkl and fourth order elastic compliance tensor S ijkl are the starting point for the calculation of a number of elastic anisotropic physical properties, which include Young s modulus, shear modulus, Poisson s ratio, linear compressibility, compressional and shear elastic wave velocities, wavefront velocities, mean sound velocities, Debye temperature, and, of course, of their isotropic equivalents. In the following we shall give a short overview over these properties. Scalar volume compressibility. First we consider the scalar volume compressibility β. Using the fact that the change of volume is given in terms of the strain tensor ε ij by V V = ε ii, 18
19 we derive for hydrostatic or isotropic pressure, which is given by the stress tensor σ kl = P δ kl, that the change of volume is given by Hence, the volume compressibility is V V = P S iikk. β = V V 1 P = S iikk. Linear compressibility. The linear compressibility β(x) of a crystal is the strain, i.e. the relative change in length l, for a specific crystallographic direction x, when the crystal l is subjected to a unit change in hydrostatic pressure P δ kl. From we conclude l l = ε ij x i x j = P S iikk x i x j β(x) = l l 1 P = S ijkkx i x j. Youngs modulus. The Young s modulus E is the ratio of the axial (longitudinal) stress to the lateral (transverse) strain in a tensile or compressive test. As we have seen earlier when discussing the elastic stiffness tensor, this type of uniaxial stress is accompanied by lateral and shear strains as well as the axial strain. The Young s modulus in direction x is given by E(x) = (S ijkl x i x j x k x l ) 1. Shear modulus. Unlike Young s modulus, the shear modulus G in an anisotropic medium is defined using two directions; the shear plane h and the shear direction u. For example, if the shear stress σ 12 results in the shear strain 2ε 12. Then the corresponding shear modulus is G = σ 12 2ε 12. From Hooke s law we have ε 12 = S 1212 σ 12 + S 1221 σ 21, hence G = (4S 1212 ) 1. The shear modulus for an arbitrary, but orthogonal, shear plane h and shear direction u is given by G(h, u) = (4S ijkl h i u j h k u l ) Poisson s Ratio. Anisotropic Poisson s ratio is defined by the elastic strain in two orthogonal directions, the longitudinal (or axial) direction x and the transverse (or lateral) direction y. The lateral strain is defined by ε ij y i y j along y and the longitudinal strain by ε ij x i x j along x. The anisotropic Poisson s ratio ν(x,y) is given as the ratio of lateral to longitudinal strain (Sirotin and Shakolskaya, 1982) as 19
20 ν(x, y) = ε ij y i y j ε kl x k x l = S ijkl x i x j y k y l S mnop x m x n x o x p. The anisotropic Poisson s ratio has recently been reported for talc (Mainprice et al., 2008) and has been found to be negative for many directions at low pressure. Wave velocities. The Christoffel equation, first published by Christoffel (1877), can be used to calculate elastic wave velocities and the polarizations in an anisotropic elastic medium from the elastic stiffness tensor C ijkl, or, more straightforward, from the Christoffel tensor T ik which is for a unit propagation direction n defined by T ik ( n) = C ijkl n j n l. Since the elastic tensors are symmetric, we have T ik ( n) = C ijkl n j n l = C jikl n j n l = C ijlk n j n l = C klij n j n l = T ki ( n), and, hence, the Christoffel tensor T ( n) is symmetric. The Christoffel tensor is also invariant upon the change of sign of the propagation direction as the elastic tensor is not sensitive to the presence or absence of a center of crystal symmetry, being a centrosymmetric physical property. Because the elastic strain energy 1/2C ijkl ε ij ε kl of a stable crystal is always positive and real (e.g. Nye, 1985), the eigenvalues λ 1, λ 1, λ 3 of the Christoffel tensor T ik ( n) are real and positive. They are related to the wave velocities V p, V s1 and V s2 of the plane P, S1 and S2 waves propagating in the direction n by the formulae λ 1 V p = ρ, V λ 2 s1 = ρ, V λ 3 s2 = ρ, where ρ denotes the material density. The three eigenvectors of the Christoffel tensor are the polarization directions, also called vibration, particle movement or displacement vectors, of the three waves. As the Christoffel tensor is symmetric the three polarization directions are mutually perpendicular. In the most general case there are no particular angular relationships between polarization directions p and the propagation direction n. However, typically, the Pwave polarization direction is nearly parallel and the two Swaves polarizations are nearly perpendicular to the propagation direction. They are termed quasi P or quasis waves. The S wave velocities may be identified unambiguously by their relative velocity V s1 > V s2. All the elastic properties mentioned in this section have direct expressions in MTEX, i.e., there are the commands b e t a = volumecompressibility (C) b e t a = linearcompressibility (C, x ) E = YoungsModulus(C, x ) G = shearmodulus(c, h, u ) nu = PoissonRatio (C, x, y ) T = ChristoffelTensor (C, n ) 20
21 Note, that all these commands take the compliance tensor C as basis for the calculations. For the calculation of the wave velocities the command velocity [ vp, vs1, vs2, pp, ps1, ps2 ] = velocity (C, x, rho ) allows for the computation of the wave velocities and the corresponding polarization directions. 3.4 Visualization In order to visualize the above quantities, MTEX offers a simple, yet flexible, syntax. Let us demonstrate it using the Talc example of the previous section. In order to plot the linear compressibility β( x) or Young s Modulus E( x) as a function of the direction x one uses the commands plot (C, PlotType, l i n e a r C o m p r e s s i b i l i t y ) plot (C, PlotType, YoungsModulus ) The resulting plots are shown in Figure 2. X X Y Z Y Z min: max: min: 17 max: Figure 2: The linear compressibility in GPa 1 (left plot) and Young s modulus in GPa (right plot) for Talc Next we want to visualize the wave velocities and the polarization directions. Let us start with the Pwave velocity in kms 1 which is plotted by rho = ; plot (C, PlotType, v e l o c i t y, vp, d e n s i t y, rho ) Note that we had to pass the density rho in gcm 3 to the plot command. Next we want to add on top of this plot the Pwave polarization directions. Therefore, we use the command hold on and hold off to prevent MTEX from clearing the output window, hold on plot (C, PlotType, v e l o c i t y, pp, d e n s i t y, rho ) ; hold o f f 21
22 The result is shown in Figure 3. Instead of only specifying the variables to plot, one can also perform simple calculations. For example by writing plot (C, PlotType, v e l o c i t y, 200 ( vs1 vs2 ). / ( vs1+vs2 ), d e n s i t y, rho ) ; hold on plot (C, PlotType, v e l o c i t y, ps1, d e n s i t y, rho ) ; hold o f f the Swave anisotropy in percent is plotted together with the polarization directions of the fastest Swave ps1. Another example illustrating the flexibility of the system is the following plot of the velocity ratio V p /V s1 together with the S1wave polarizations direction. plot (C, PlotType, v e l o c i t y, vp. / vs1, d e n s i t y, rho ) ; hold on plot (C, PlotType, v e l o c i t y, ps1, d e n s i t y, rho ) ; hold o f f min: 3.94 (a) Pwave velocity max: 9.1 min: 0.2 (b) Swave anisotropy max: 86 min: 1 (c) Vp/Vs1 ratio max: 1.7 Figure 3: Wave velocities of a Talc crystal. Figure (a) shows the Pwave velocity together with the Pwave polarization direction. Figure (b) shows the Swave anisotropy in percent together with the S1wave polarization direction, whereas Figure (c) shows the ratio of Vp/Vs1 velocities together with the S1wave polarization direction Anisotropic properties of polyphase aggregates In this section we are concerned with the problem of calculating average physical properties of polyphase aggregates. To this end two ingredients are required for each phase p: 1. the property tensor T p i 1,...,i r reference orientation, describing the physical behavior of a single crystal in the the orientation density function (ODF) f p (g) describing the volume portion V V crystals having orientation g, of 22
23 or a representative set of individual orientations g m, m = 1,..., M, for example measured by EBSD. As an example we consider an aggregate composed of two minerals, Glaucophane and Epidote using data from a Blue Schist. The corresponding crystal reference frames are defined by cs Glaucophane = symmetry( 2/m, [ , , ], [ , , ] degree, mineral, Glaucophane ) ; c s E p i d o t e = symmetry( 2/m, [ , , ], [ , , ] degree, mineral, Epidote ) ; For Glaucophane the elastic stiffness was measured by Bezacier et al. (2010) who give the tensor C_ Glaucophane = tensor ( size : ) rank : 4 mineral : Glaucophane (2/m, X a*, Y b, Z c) tensor in Voigt matrix representation and for Epidote the elastic stiffness was measured by Alexsandrov et al. (1974) who gives the tensor C_ Epidote = tensor ( size : ) rank : 4 mineral : Epidote (2/m, X a*, Y b, Z c) tensor in Voigt matrix representation Computing the average tensor from individual orientations We start with the case that we have individual orientation data g m, m = 1,..., M, i.e., from EBSD or Ustage measurements, and volume fractions V m, m = 1,..., M. Then the bestknown averaging techniques for obtaining estimates of the effective properties of aggregates are those developed for elastic constants by Voigt (1887,1928) and Reuss 23
24 (1929). The Voigt average is defined by assuming that the induced tensor (in broadest sense including vectors) field is everywhere homogeneous or constant, i.e., the induced tensor at every position is set equal to the macroscopic induced tensor of the specimen. In the classical example of elasticity the strain field is considered constant.the Voigt average is sometimes called the series average by analogy with Ohms law for electrical circuits. The Voigt average specimen effective tensor T Voigt is defined by the volume average of the individual tensors T (gm) c with crystal orientations gm c and volume fractions V m, T Voigt = M V m T (gm). c m=1 Contrarily, the Reuss average is defined by assuming that the applied tensor field is everywhere constant, i.e., the applied tensor at every position is set equal to the macroscopic applied tensor of the specimen. In the classical example of elasticity the stress field is considered constant.the Reuss average is sometimes called the parallel average. The specimen effective tensor T Reuss is defined by the volume ensemble average of the inverses of the individual tensors T 1 (gm), c [ M 1 T Reuss = V m T 1 (gm)] c. m=1 The experimentally measured tensor of aggregates is in general between the Voigt and Reuss average bounds as the applied and induced tensor fields distributions are expected to be between uniform induced (Voigt bound) and uniform applied (Reuss bound) field limits. Hill (1952) observed that the arithmetic mean of the Voigt and Reuss bounds T Hill = 1 2 ( T Voigt + T Reuss), sometimes called the Hill or VoigtReussHill (VRH) average, is often close to experimental values for the elastic fourth order tensor. Although VRH average has no theoretical justification, it is widely used in earth and materials sciences. In the example outlined above of an aggregate consisting of Glaucophane and Epidote we consider an EBSD data set measured by Bezacier et al. (2010). In MTEX such individual orientation data are represented by a variable of type EBSD which is generated from an ASCII file containing the individual orientation measurements by the command ebsd = loadebsd ( FileName,{ cs Glaucophane, c s E p i d o t e }) ebsd = EBSD ( Groix_A50_5_stitched. ctf ) properties : bands, bc, bs, error, mad phase orientations mineral symmetry crystal reference frame Glaucophane 2/m X a*, Y b, Z c Epidote 2/m X a*, Y b, Z c 24
Understand basic stressstrain response of engineering materials.
Module 3 Constitutive quations Learning Objectives Understand basic stressstrain response of engineering materials. Quantify the linear elastic stressstrain response in terms of tensorial quantities
More informationContinuum mechanics V. Constitutive equations. 1. Constitutive equation: definition and basic axioms
Continuum mechanics office Math 0.107 ales.janka@unifr.ch http://perso.unifr.ch/ales.janka/mechanics Mars 16, 2011, Université de Fribourg 1. Constitutive equation: definition and basic axioms Constitutive
More informationMATERIAL MECHANICS, SE2126 COMPUTER LAB 4 MICRO MECHANICS. E E v E E E E E v E E + + = m f f. f f
MATRIAL MCHANICS, S226 COMPUTR LAB 4 MICRO MCHANICS 2 2 2 f m f f m T m f m f f m v v + + = + PART A SPHRICAL PARTICL INCLUSION Consider a solid granular material, a so called particle composite, shown
More information3D and Planar Constitutive Relations
3D and Planar Constitutive Relations A School on Mechanics of Fibre Reinforced Polymer Composites Knowledge Incubation for TEQIP Indian Institute of Technology Kanpur PM Mohite Department of Aerospace
More informationIntroduction to Seismology Spring 2008
MIT OpenCourseWare http://ocw.mit.edu 12.510 Introduction to Seismology Spring 2008 For information about citing these materials or our Terms of Use, visit: http://ocw.mit.edu/terms. Stress and Strain
More informationContinuum Mechanics. Continuum Mechanics and Constitutive Equations
Continuum Mechanics Continuum Mechanics and Constitutive Equations Continuum mechanics pertains to the description of mechanical behavior of materials under the assumption that the material is a uniform
More informationBasic concepts to start Mechanics of Materials
Basic concepts to start Mechanics of Materials Georges Cailletaud Centre des Matériaux Ecole des Mines de Paris/CNRS Notations Notations (maths) (1/2) A vector v (element of a vectorial space) can be seen
More informationStressinduced transverse isotropy in rocks
Stanford Exploration Project, Report 80, May 15, 2001, pages 1 318 Stressinduced transverse isotropy in rocks Lawrence M. Schwartz, 1 William F. Murphy, III, 1 and James G. Berryman 1 ABSTRACT The application
More informationResource reading (If you would like to brush up on stress, strain, and elasticity):
12.108 Struct. & Prop s. of Earth Mat. Lecture 9 1 Singlecrystal elasticity Assigned Reading: Nye JF (1957) Physical Properties of Crystals. Oxford University Press, Oxford, UK (Chapters 5 and 6). Nye,
More informationTextures in experimentally deformed olivine aggregates: the effects of added water and melt.
Textures in experimentally deformed olivine aggregates: the effects of added water and melt. F. Heidelbach 1, a, B. Holtzman 2, b, S. HierMajumder 2, c and D. Kohlstedt 2, d 1 Bayerisches Geoinstitut,
More informationAttenuation of ultrasonic waves in rolled metals
University of Nebraska  Lincoln DigitalCommons@University of Nebraska  Lincoln Faculty Publications from Nebraska Center for Materials and Nanoscience Materials and Nanoscience, Nebraska Center for (NCMN)
More informationChapter 16: Elastic Solids
Chapter 16: Elastic Solids Chapter 16: Elastic Solids... 366 16.1 Introduction... 367 16.2 The Elastic Strain... 368 16.2.1 The displacement vector... 368 16.2.2 The deformation gradient... 368 16.2.3
More informationStructure and Dynamics : An Atomic View of Materials
Structure and Dynamics : An Atomic View of Materials MARTIN T. DOVE Department ofearth Sciences University of Cambridge OXFORD UNIVERSITY PRESS Contents 1 Introduction 1 1.1 Observations 1 1.1.1 Microscopic
More informationReference material Reference books: Y.C. Fung, "Foundations of Solid Mechanics", Prentice Hall R. Hill, "The mathematical theory of plasticity",
Reference material Reference books: Y.C. Fung, "Foundations of Solid Mechanics", Prentice Hall R. Hill, "The mathematical theory of plasticity", Oxford University Press, Oxford. J. Lubliner, "Plasticity
More informationElements of Rock Mechanics
Elements of Rock Mechanics Stress and strain Creep Constitutive equation Hooke's law Empirical relations Effects of porosity and fluids Anelasticity and viscoelasticity Reading: Shearer, 3 Stress Consider
More informationEffects of Fracture Parameters in an Anisotropy Model on PWave Azimuthal Amplitude Responses
PROC. ITB Eng. Science Vol. 38 B, No. 2, 2006, 159170 159 Effects of Fracture Parameters in an Anisotropy Model on PWave Azimuthal Amplitude Responses Fatkhan Program Studi Teknik Geofisika FIKTMITB
More informationResidual Stress analysis
Residual Stress analysis Informations: strains Macro elastic strain tensor (I kind) Crystal anisotropic strains (II kind) Fe Cu C Macro and micro stresses Applied macro stresses Residual Stress/Strain
More informationAn acoustic wave equation for orthorhombic anisotropy
Stanford Exploration Project, Report 98, August 1, 1998, pages 6?? An acoustic wave equation for orthorhombic anisotropy Tariq Alkhalifah 1 keywords: Anisotropy, finite difference, modeling ABSTRACT Using
More informationSolid State Theory Physics 545
olid tate Theory hysics 545 Mechanical properties of materials. Basics. tress and strain. Basic definitions. Normal and hear stresses. Elastic constants. tress tensor. Young modulus. rystal symmetry and
More informationGeology 229 Engineering Geology. Lecture 5. Engineering Properties of Rocks (West, Ch. 6)
Geology 229 Engineering Geology Lecture 5 Engineering Properties of Rocks (West, Ch. 6) Common mechanic properties: Density; Elastic properties:  elastic modulii Outline of this Lecture 1. Uniaxial rock
More informationLecture 7. Properties of Materials
MIT 3.00 Fall 2002 c W.C Carter 55 Lecture 7 Properties of Materials Last Time Types of Systems and Types of Processes Division of Total Energy into Kinetic, Potential, and Internal Types of Work: Polarization
More informationMECHANICS OF MATERIALS. EQUATIONS AND THEOREMS
1 MECHANICS OF MATERIALS. EQUATIONS AND THEOREMS Version 20110114 Stress tensor Definition of traction vector (1) Cauchy theorem (2) Equilibrium (3) Invariants (4) (5) (6) or, written in terms of principal
More informationModule 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationSurface stress and relaxation in metals
J. Phys.: Condens. Matter 12 (2000) 5541 5550. Printed in the UK PII: S09538984(00)113864 Surface stress and relaxation in metals P M Marcus, Xianghong Qian and Wolfgang Hübner IBM Research Center, Yorktown
More informationCopyright(c)JCPDSInternational Centre for Diffraction Data 2000,Advances in Xray Analysis,Vol ISSN
Copyright(c)JCPDSInternational Centre for Diffraction Data 2000,Advances in Xray Analysis,Vol.43 129 MATHEMATICAL OF DIFFRACTION PROPERTIES POLE FIGURES ABSTRACT Helmut Schaeben Mathematics and Computer
More information6.730 Physics for Solid State Applications
6.730 Physics for Solid State Applications Lecture 5: Specific Heat of Lattice Waves Outline Review Lecture 4 3D Elastic Continuum 3D Lattice Waves Lattice Density of Modes Specific Heat of Lattice Specific
More informationTensor Visualization. CSC 7443: Scientific Information Visualization
Tensor Visualization Tensor data A tensor is a multivariate quantity Scalar is a tensor of rank zero s = s(x,y,z) Vector is a tensor of rank one v = (v x,v y,v z ) For a symmetric tensor of rank 2, its
More informationA Constitutive Framework for the Numerical Analysis of Organic Soils and Directionally Dependent Materials
Dublin, October 2010 A Constitutive Framework for the Numerical Analysis of Organic Soils and Directionally Dependent Materials FracMan Technology Group Dr Mark Cottrell Presentation Outline Some Physical
More informationInstitute de Physique du Globe, Paris, France. Summary
Laboratory determination of velocity anisotropy Jason Z. Han, Douglas R. Schmitt, Daniel Collis a, and Javier Escartin b a Institute for Geophysical Research, Department of Physics, University of Alberta,
More informationIn this section, thermoelasticity is considered. By definition, the constitutive relations for Gradθ. This general case
Section.. Thermoelasticity In this section, thermoelasticity is considered. By definition, the constitutive relations for F, θ, Gradθ. This general case such a material depend only on the set of field
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationSymmetry. 2D Symmetry. 2D Symmetry. Symmetry. EESC 2100: Mineralogy 1. Symmetry Elements 1. Rotation. Symmetry Elements 1. Rotation.
Symmetry a. Twofold rotation = 30 o /2 rotation a. Twofold rotation = 30 o /2 rotation Operation Motif = the symbol for a twofold rotation EESC 2100: Mineralogy 1 a. Twofold rotation = 30 o /2 rotation
More informationLectures on. Constitutive Modelling of Arteries. Ray Ogden
Lectures on Constitutive Modelling of Arteries Ray Ogden University of Aberdeen Xi an Jiaotong University April 2011 Overview of the Ingredients of Continuum Mechanics needed in Soft Tissue Biomechanics
More informationUNIT I SOLID STATE PHYSICS
UNIT I SOLID STATE PHYSICS CHAPTER 1 CRYSTAL STRUCTURE 1.1 INTRODUCTION When two atoms are brought together, two kinds of forces: attraction and repulsion come into play. The force of attraction increases
More informationPEAT SEISMOLOGY Lecture 9: Anisotropy, attenuation and anelasticity
PEAT8002  SEISMOLOGY Lecture 9: Anisotropy, attenuation and anelasticity Nick Rawlinson Research School of Earth Sciences Australian National University Anisotropy Introduction Most of the theoretical
More informationPiezo materials. Actuators Sensors Generators Transducers. Piezoelectric materials may be used to produce e.g.: Piezo materials Ver1404
Noliac Group develops and manufactures piezoelectric materials based on modified lead zirconate titanate (PZT) of high quality and tailored for custom specifications. Piezoelectric materials may be used
More information1.103 CIVIL ENGINEERING MATERIALS LABORATORY (123) Dr. J.T. Germaine Spring 2004 LABORATORY ASSIGNMENT NUMBER 6
1.103 CIVIL ENGINEERING MATERIALS LABORATORY (123) Dr. J.T. Germaine MIT Spring 2004 LABORATORY ASSIGNMENT NUMBER 6 COMPRESSION TESTING AND ANISOTROPY OF WOOD Purpose: Reading: During this laboratory
More informationP314 Anisotropic Elastic Modelling for Organic Shales
P314 Anisotropic Elastic Modelling for Organic Shales X. Wu* (British Geological Survey), M. Chapman (British Geological Survey), X.Y. Li (British Geological Survey) & H. Dai (British Geological Survey)
More informationBy drawing Mohr s circle, the stress transformation in 2D can be done graphically. + σ x σ y. cos 2θ + τ xy sin 2θ, (1) sin 2θ + τ xy cos 2θ.
Mohr s Circle By drawing Mohr s circle, the stress transformation in D can be done graphically. σ = σ x + σ y τ = σ x σ y + σ x σ y cos θ + τ xy sin θ, 1 sin θ + τ xy cos θ. Note that the angle of rotation,
More informationWave Propagation in Anisotropic, Anelastic, Porous and Electromagnetic Media
SECTION I. SEISMIC EXPLORATION Volume 38 WAVE FIELDS IN REAL MEDIA: Wave Propagation in Anisotropic, Anelastic, Porous and Electromagnetic Media (SECOND EDITION, REVISED AND EXTENDED) by Jose M. CARCIONE
More information. D CR Nomenclature D 1
. D CR Nomenclature D 1 Appendix D: CR NOMENCLATURE D 2 The notation used by different investigators working in CR formulations has not coalesced, since the topic is in flux. This Appendix identifies the
More informationAnisotropic modeling of short fibers reinforced thermoplastics materials with LSDYNA
Anisotropic modeling of short fibers reinforced thermoplastics materials with LSDYNA Alexandre Hatt 1 1 Faurecia Automotive Seating, Simplified Limited Liability Company 1 Abstract / Summary Polymer thermoplastics
More informationChap. 4. Electromagnetic Propagation in Anisotropic Media
Chap. 4. Electromagnetic Propagation in Anisotropic Media  Optical properties depend on the direction of propagation and the polarization of the light.  Crystals such as calcite, quartz, KDP, and liquid
More informationEarth Materials Lab 2  Lattices and the Unit Cell
Earth Materials Lab 2  Lattices and the Unit Cell Unit Cell Minerals are crystallographic solids and therefore are made of atoms arranged into lattices. The average size hand specimen is made of more
More informationGame Physics. Game and Media Technology Master Program  Utrecht University. Dr. Nicolas Pronost
Game and Media Technology Master Program  Utrecht University Dr. Nicolas Pronost Soft body physics Soft bodies In reality, objects are not purely rigid for some it is a good approximation but if you hit
More information3.091 Introduction to Solid State Chemistry. Lecture Notes No. 5a ELASTIC BEHAVIOR OF SOLIDS
3.091 Introduction to Solid State Chemistry Lecture Notes No. 5a ELASTIC BEHAVIOR OF SOLIDS 1. INTRODUCTION Crystals are held together by interatomic or intermolecular bonds. The bonds can be covalent,
More informationMethane hydrate rock physics models for the Blake Outer Ridge
Stanford Exploration Project, Report 80, May 15, 2001, pages 1 307 Methane hydrate rock physics models for the Blake Outer Ridge Christine Ecker 1 ABSTRACT Seismic analyses of methane hydrate data from
More informationMATERIAL ELASTIC ANISOTROPIC command
MATERIAL ELASTIC ANISOTROPIC command.. Synopsis The MATERIAL ELASTIC ANISOTROPIC command is used to specify the parameters associated with an anisotropic linear elastic material idealization. Syntax The
More informationSymmetry Crystallography
Crystallography Motif: the fundamental part of a symmetric design that, when repeated, creates the whole pattern In 3D, translation defines operations which move the motif into infinitely repeating patterns
More informationRoad map (Where are we headed?)
Road map (Where are we headed?) oal: Fairly high level understanding of carrier transport and optical transitions in semiconductors Necessary Ingredients Crystal Structure Lattice Vibrations Free Electron
More informationAnisotropy of Shale Properties: A MultiScale and MultiPhysics Characterization
Observation Scale Wavelength 10 0 10 4 10 6 10 8 10 12 10 16 10 18 10 20 Frequency (Hz) Anisotropy of Shale Properties: A MultiScale and MultiPhysics Characterization Elastic, Mechanical, Petrophysical
More informationCONSTITUTIVE RELATIONS FOR LINEAR ELASTIC SOLIDS
Chapter 9 CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS Figure 9.1: Hooke memorial window, St. Helen s, Bishopsgate, City of London 211 212 CHAPTR 9. CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS 9.1 Mechanical
More informationNumerical Modeling for Different Types of Fractures
umerical Modeling for Different Types of Fractures Xiaoqin Cui* CREWES Department of Geoscience University of Calgary Canada xicui@ucalgary.ca and Laurence R. Lines Edward S. Krebes Department of Geoscience
More informationAnalysis of high loss viscoelastic composites
Analysis of high loss viscoelastic composites by C. P. Chen, Ph.D. and R. S. Lakes, Ph.D. Department of Engineering Physics Engineering Mechanics Program; Biomedical Engineering Department Materials Science
More informationModelling Anisotropic, Hyperelastic Materials in ABAQUS
Modelling Anisotropic, Hyperelastic Materials in ABAQUS Salvatore Federico and Walter Herzog Human Performance Laboratory, Faculty of Kinesiology, The University of Calgary 2500 University Drive NW, Calgary,
More informationThe structure of liquids and glasses. The lattice and unit cell in 1D. The structure of crystalline materials. Describing condensed phase structures
Describing condensed phase structures Describing the structure of an isolated small molecule is easy to do Just specify the bond distances and angles How do we describe the structure of a condensed phase?
More informationQ. WANG, QK. XIA, S. Y. O REILLY, W. L. GRIFFIN, E. E. BEYER AND H. K. BRUECKNER
Pressure and stressinduced fabric transition in olivine from peridotites in the Western Gneiss Region (Norway): implications for mantle seismic anisotropy Q. WANG, QK. XIA, S. Y. O REILLY, W. L. GRIFFIN,
More informationIntroduction to Continuous Systems. Continuous Systems. Strings, Torsional Rods and Beams.
Outline of Continuous Systems. Introduction to Continuous Systems. Continuous Systems. Strings, Torsional Rods and Beams. Vibrations of Flexible Strings. Torsional Vibration of Rods. BernoulliEuler Beams.
More informationTuesday, February 11, Chapter 3. Load and Stress Analysis. Dr. Mohammad Suliman Abuhaiba, PE
1 Chapter 3 Load and Stress Analysis 2 Chapter Outline Equilibrium & FreeBody Diagrams Shear Force and Bending Moments in Beams Singularity Functions Stress Cartesian Stress Components Mohr s Circle for
More informationList of Comprehensive Exams Topics
List of Comprehensive Exams Topics Mechanics 1. Basic Mechanics Newton s laws and conservation laws, the virial theorem 2. The Lagrangian and Hamiltonian Formalism The Lagrange formalism and the principle
More informationEE C245 ME C218 Introduction to MEMS Design
EE C245 ME C218 Introduction to MEMS Design Fall 2007 Prof. Clark T.C. Nguyen Dept. of Electrical Engineering & Computer Sciences University of California at Berkeley Berkeley, CA 94720 Lecture 16: Energy
More information2. Mechanics of Materials: Strain. 3. Hookes's Law
Mechanics of Materials Course: WB3413, Dredging Processes 1 Fundamental Theory Required for Sand, Clay and Rock Cutting 1. Mechanics of Materials: Stress 1. Introduction 2. Plane Stress and Coordinate
More informationDESIGN OF LAMINATES FOR INPLANE LOADING
DESIGN OF LAMINATES FOR INPLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, 72000 Le Mans, France Georges.Verchery@m4x.org SUMMARY This work relates to the design of laminated structures primarily
More informationMagnetohydrodynamic waves in a plasma
Department of Physics Seminar 1b Magnetohydrodynamic waves in a plasma Author: Janez Kokalj Advisor: prof. dr. Tomaž Gyergyek Petelinje, April 2016 Abstract Plasma can sustain different wave phenomena.
More informationChapter 2. Rubber Elasticity:
Chapter. Rubber Elasticity: The mechanical behavior of a rubber band, at first glance, might appear to be Hookean in that strain is close to 100% recoverable. However, the stress strain curve for a rubber
More informationRoger Johnson Structure and Dynamics: Displacive phase transition Lecture 9
9.1. Summary In this Lecture we will consider structural phase transitions characterised by atomic displacements, which result in a low temperature structure that is distorted compared to a higher temperature,
More informationChapter 6: Mechanical Properties of Metals. Dr. Feras Fraige
Chapter 6: Mechanical Properties of Metals Dr. Feras Fraige Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility Toughness
More informationCHARACTERIZATION OF SATURATED POROUS ROCKS WITH OBLIQUELY DIPPING FRACTURES. Jiao Xue and Robert H. Tatham
CHARACTERIZATION OF SATURATED POROUS ROCS WITH OBLIQUELY DIPPING FRACTURES Jiao Xue and Robert H. Tatham Department of Geological Sciences The University of Texas at Austin ABSTRACT Elastic properties,
More informationNMR Shifts. I Introduction and tensor/crystal symmetry.
NMR Shifts. I Introduction and tensor/crystal symmetry. These notes were developed for my group as introduction to NMR shifts and notation. 1) Basic shift definitions and notation: For nonmagnetic materials,
More informationDEVELOPMENT OF A CONTINUUM PLASTICITY MODEL FOR THE COMMERCIAL FINITE ELEMENT CODE ABAQUS
DEVELOPMENT OF A CONTINUUM PLASTICITY MODEL FOR THE COMMERCIAL FINITE ELEMENT CODE ABAQUS Mohsen Safaei, Wim De Waele Ghent University, Laboratory Soete, Belgium Abstract The present work relates to the
More informationCellular solid structures with unbounded thermal expansion. Roderic Lakes. Journal of Materials Science Letters, 15, (1996).
1 Cellular solid structures with unbounded thermal expansion Roderic Lakes Journal of Materials Science Letters, 15, 475477 (1996). Abstract Material microstructures are presented which can exhibit coefficients
More informationProceedings of the ASME th International Conference on Ocean, Offshore and Arctic Engineering OMAE2016 June 1924, 2016, Busan, South Korea
Proceedings of the ASME 26 35th International Conference on Ocean, Offshore and Arctic Engineering OMAE26 June 924, 26, Busan, South Korea OMAE2654554 LOCAL STRAIN AND STRESS CALCULATION METHODS OF IRREGULAR
More informationA PAPER ON DESIGN AND ANALYSIS OF PRESSURE VESSEL
A PAPER ON DESIGN AND ANALYSIS OF PRESSURE VESSEL P.Palanivelu 1, R.Siva Prasad 2, 1 PG Scholar, Department of Mechanical Engineering, Gojan School of Business and Technology, Redhills, Chennai, India.
More informationElastic Properties of Polycrystalline Solid Helium
JLowTempPhys(2010)160:5 11 DOI 10.1007/s1090901001738 Elastic Properties of Polycrystalline Solid Helium Humphrey J. Maris Sebastien Balibar Received: 29 March 2010 / Accepted: 16 April 2010 / Published
More informationEffective Medium Theories Effective Medium Models
Effective Medium Models 3 Bounding Methods for Estimating Effective Elastic Moduli For many reasons we would like to be able to model or estimate the effective elastic moduli of rocks in terms of the properties
More informationBasic Concepts of Strain and Tilt. Evelyn Roeloffs, USGS June 2008
Basic Concepts of Strain and Tilt Evelyn Roeloffs, USGS June 2008 1 Coordinates Righthanded coordinate system, with positions along the three axes specified by x,y,z. x,y will usually be horizontal, and
More information5 Symmetries and point group in a nut shell
30 Phys520.nb 5 Symmetries and point group in a nut shell 5.1. Basic ideas: 5.1.1. Symmetry operations Symmetry: A system remains invariant under certain operation. These operations are called symmetry
More informationThe Power of Ultrasonic Characterisation for Completely Assessing the Elastic Properties of Materials
11th European Conference on NonDestructive Testing (ECNDT 214), October 61, 214, Prague, Czech Republic The Power of Ultrasonic Characterisation for Completely Assessing the Elastic Properties of Materials
More information**********************************************************************
Department of Civil and Environmental Engineering School of Mining and Petroleum Engineering 333 Markin/CNRL Natural Resources Engineering Facility www.engineering.ualberta.ca/civil Tel: 780.492.4235
More information2.1 Strain energy functions for incompressible materials
Chapter 2 Strain energy functions The aims of constitutive theories are to develop mathematical models for representing the real behavior of matter, to determine the material response and in general, to
More informationChapter 5. Effects of Photonic Crystal Band Gap on Rotation and Deformation of Hollow Te Rods in Triangular Lattice
Chapter 5 Effects of Photonic Crystal Band Gap on Rotation and Deformation of Hollow Te Rods in Triangular Lattice In chapter 3 and 4, we have demonstrated that the deformed rods, rotational rods and perturbation
More informationThe Basic Properties of Surface Waves
The Basic Properties of Surface Waves Lapo Boschi lapo@erdw.ethz.ch April 24, 202 Love and Rayleigh Waves Whenever an elastic medium is bounded by a free surface, coherent waves arise that travel along
More informationME 582 Advanced Materials Science. Chapter 2 Macromechanical Analysis of a Lamina (Part 2)
ME 582 Advanced Materials Science Chapter 2 Macromechanical Analysis of a Lamina (Part 2) Laboratory for Composite Materials Research Department of Mechanical Engineering University of South Alabama, Mobile,
More informationELASTICITY (MDM 10203)
LASTICITY (MDM 10203) Lecture Module 5: 3D Constitutive Relations Dr. Waluyo Adi Siswanto University Tun Hussein Onn Malaysia Generalised Hooke's Law In one dimensional system: = (basic Hooke's law) Considering
More informationPlane Strain Test for Metal Sheet Characterization
Plane Strain Test for Metal Sheet Characterization Paulo Flores 1, Felix Bonnet 2 and AnneMarie Habraken 3 1 DIM, University of Concepción, Edmundo Larenas 270, Concepción, Chile 2 ENS  Cachan, Avenue
More informationTransduction Based on Changes in the Energy Stored in an Electrical Field
Lecture 71 Transduction Based on Changes in the Energy Stored in an Electrical Field  Electrostriction The electrostrictive effect is a quadratic dependence of strain or stress on the polarization P
More informationStress induced seismic velocity anisotropy study Bin Qiu, Mita Sengupta, Jorg Herwanger, WesternGeco/Schlumberger
anisotropy study Bin Qiu, Mita Sengupta, Jorg Herwanger, WesternGeco/Schlumberger Summary A method of calculating stress induced seismic velocity anisotropy is presented and studied. In a first step an
More informationBasic Energy Principles in Stiffness Analysis
Basic Energy Principles in Stiffness Analysis StressStrain Relations The application of any theory requires knowledge of the physical properties of the material(s) comprising the structure. We are limiting
More informationAppendix A: Crystal Symmetries and Elastic Constants. A.1 Crystal Classes, Point Groups, and Laue Groups
Appendix A: Crystal Symmetries and Elastic Constants In anisotropic materials, constitutive relations and corresponding material coefficients depend on the orientation of the body with respect to the reference
More informationMathematical Modeling of Displacements and Thermal Stresses in Anisotropic Materials (Sapphire) in Cooling
Mathematical Modeling of Displacements and Thermal Stresses in Anisotropic Materials (Sapphire) in Cooling Timo Tiihonen & Tero Tuovinen September 11, 2015 European Study Group with Industry, ESGI 112,
More informationPlane and axisymmetric models in Mentat & MARC. Tutorial with some Background
Plane and axisymmetric models in Mentat & MARC Tutorial with some Background Eindhoven University of Technology Department of Mechanical Engineering Piet J.G. Schreurs Lambèrt C.A. van Breemen March 6,
More informationLecture 13: Tensors in paleomagnetism. What are tensors anyway? anisotropy of magnetic susceptibility (AMS) how to find it. what to do with it
Lecture 13: Tensors in paleomagnetism What are tensors anyway? anisotropy of magnetic susceptibility (AMS) how to find it what to do with it anisotropy of magnetic remanence 1 What is a tensor? An array
More informationChapter 11. Special Relativity
Chapter 11 Special Relativity Note: Please also consult the fifth) problem list associated with this chapter In this chapter, Latin indices are used for space coordinates only eg, i = 1,2,3, etc), while
More information6. Bending CHAPTER OBJECTIVES
CHAPTER OBJECTIVES Determine stress in members caused by bending Discuss how to establish shear and moment diagrams for a beam or shaft Determine largest shear and moment in a member, and specify where
More informationCE570 Advanced Structural Mechanics  Arun Prakash
Ch1Intro Page 1 CE570 Advanced Structural Mechanics  Arun Prakash The BIG Picture What is Mechanics? Mechanics is study of how things work: how anything works, how the world works! People ask: "Do you
More informationModule 2: Thermal Stresses in a 1D Beam Fixed at Both Ends
Module 2: Thermal Stresses in a 1D Beam Fixed at Both Ends Table of Contents Problem Description 2 Theory 2 Preprocessor 3 Scalar Parameters 3 Real Constants and Material Properties 4 Geometry 6 Meshing
More informationCHAPTER: 8. ELECTRONIC STRUCTURE AND ELASTIC PROPERTIES OF CrC AND CrN. 8.1 Introduction. Ph.D. Thesis: J. Maibam
CHAPTER 8 CHAPTER: 8 ELECTRONIC STRUCTURE AND ELASTIC PROPERTIES OF CrC AND CrN 8.1 Introduction In this chapter, we have selected CrC and CrN from group VIB transition metal carbides and nitrides for
More informationGeophysical Journal International
Geophysical Journal International Geophys. J. Int. (2011) 185, 609 621 doi: 10.1111/j.1365246X.2011.04978.x The influence of microstructure on seismic wave speed anisotropy in the crust: computational
More informationENGN 2290: Plasticity Computational plasticity in Abaqus
ENGN 229: Plasticity Computational plasticity in Abaqus The purpose of these exercises is to build a familiarity with using usermaterial subroutines (UMATs) in Abaqus/Standard. Abaqus/Standard is a finiteelement
More information